Comparison of different adhesive techniques using a universal adhesive system
© The Author(s) 2017
Received: 25 September 2017
Accepted: 7 November 2017
Published: 25 November 2017
In order to simplify the technique while maintaining its effective clinical performance, as well as its adhesive properties, universal adhesive systems are constantly launched in the market. Thus, the objective of this study was to compare the presence or absence of moisture in the adhesion technique using a universal adhesive system, the Single Bond Universal (3M ESPE). There were selected forty-five human molars with indications for exodontia that were divided into three experimental groups: Single Bond Universal (3M ESPE) with and without moisture in the dentin; Scotchbond Multi-Bottles (3M ESPE) conventional technique (control). The characterization methods used were: microshear and scanning electron microscopy. Statistical analysis of variance analysis (single-factor ANOVA) and Tukey’s multiple comparison, global significance level of 5% were used. It was observed through the micro-test that there were no statistically significant differences between the groups tested. Scanning electron microscopy analysis showed that the most frequent failure mode was the adhesive type (91%), followed by the mixed type fracture (8%) and the cohesive type (1%). It was concluded through this study that, regardless of the moisture (present or absent), the Single Bond Universal adhesive system showed bond strength similar to the conventional adhesive.
The adhesive technique is fundamental to the clinical success of dental rehabilitation. The adhesive procedures have the purpose of promoting adhesion between the restorative material and the tooth—enamel and dentin [1–3]. The literature highlights the need to maintain a certain degree of hydration of the dentin collagen matrix, thus avoiding its collapse and providing satisfactory infiltration of the adhesive in the demineralized portion [2, 4, 5]. However, due to the complex nature of dental cavities that may present very dry or very wet regions in the same tooth, achieving optimal hydration of the substrate is extremely difficult . The excess water in the adhesion site leads to the dilution of the constituent monomers of the adhesive material, interfering in the polymerization thereof and consequently forming a low-quality hybrid layer, which can lead to a decrease in the adhesive strength of the material . The more effective drying of the demineralized dentin promotes the removal of water from the collagen fibers, preventing the formation of voids between the remaining dentin and the dentin/adhesive/composite interface, responsible for the permeability of this interface and its solubilization [5, 6]. The creation of a porous and thin hybrid layer, besides resulting in lower adhesion strength, allows the passage of residual monomers to the pulp causing irritation and sensitivity .
While the collapse of the collagen fibers caused by total water removal causes degradation of the adhesive interface and formation of tooth/composite slits, total cavity drying increases pulpal toxicity and sensitivity. Thus, several types of adhesives and techniques have been developed with the incorporation of different materials to correct or ameliorate these deleterious effects, prolonging treatment longevity .
Recently a new adhesive product, the Universal Single Bond , has been launched on the market, this adhesive system comprises in a single bottle the self-etching acid and the adhesive, and according to the manufacturer, it can be used in the adhesive preference technique of the professional. This means that the Dental Surgeon has the option of choosing the adhesive technique that favors him during the restorative procedure, be it a total acid conditioning in enamel and dentin, or a self-etching procedure or selective enamel conditioning.
The basis presented by the manufacturer , which serves as a basis for explaining the advantages offered by this adhesive system, seems to be related to the unique developed VMS technology. This technology consists of the combination of three important chemical components for the adhesion process: the Vitrebond™ Copolymer, which allows rehydration of the collagen fibers and consequent formation of the hybrid layer, allowing its use even in dry dentin. This adhesive has the MDP (10-methacryloyl oxide decyl hydrogenphosphate), which promotes better adhesion performance to the tooth substrate, improved product stability, increased adhesion in the self-etching technique, and is also used as a metal primer. The added silane allows the adhesion mechanism to occur in glass derived (feldspathic and lithium disilicate) ceramics, in the ceramics infiltrated by glass (alumina) and Lava Zirconia, without the need for application of a separate initiating agent. The Single Bond adhesive, when combined with the exclusive DCA (dual cure activator) system for cementation, also allows bonding between cements, fillers and composite resins of chemical and dual activation .
In addition to the aforementioned advantages, this adhesive system also has other significant indications, such as in direct restorations in resin or resin-modified monomers, in root desensitization, as a protective layer for restorations of glass ionomer cement, in resin restorations and in sealant and fissures without previous acid conditioning. It is also indicated in indirect adhesive restorations, allowing cementation of facets, inlays, onlays, crowns with dual cements, in intraoral repairs of indirect restorations and immediate dentin sealing .
Considering the versatility of indications and advantages offered by this adhesive, there are few studies in the literature comparing bond strength data in dentin with different adhesive techniques, therefore, the present study had as objective compare through the microshear bond test, the presence or absence of moisture in the dentin in the adhesion technique using an universal adhesive system, the Universal Single Bond (Scotch Bond Universal).
After approval by the ethics committee of the University Santo Amaro (Process No. 1.203.890), 45 healthy human third molars were selected, which were indicated for extraction and were extracted at the Surgery Clinic of the Dental School of University Santo Amaro.
The teeth were cleaned with periodontal curettes, washed in running water and stored in distilled water under refrigeration. The occlusal third of the teeth was sectioned using a diamond disc under water-cooling in a cutting machine (Isomet) to obtain an enamel free flat dentin surface. The specimens were embedded in PVC (polyvinyl chloride) tubes using acrylic resin and leaving the coronary portion out of the tube.
Considering that the factor analyzed was the moisture in the dentin in the adhesive technique (present or absent) using the adhesive system Single Bond Universal (3M ESPE), the control group was consisted of the conventional technique using the adhesive system Scotchbond Multi-purpose (3M espe). Each of the three experimental groups containing 15 teeth. The smear layer was standardized using 220-grit granulation sandpaper, rubbing the already sectioned tooth for 15 s, perpendicularly to the sandpaper [11–15].
Conventional technique using Scotchbond Multi-purpose (control)
The dentin was etched for 15 s using 37% phosphoric acid (Fusion-Duralink, Angelus) then washed with water/air spray also for 15 s. The excess water was removed with gently air jets , maintaining the moisture of the dentin. The primer (solution of resinous monomers diluted in organic solvents, which in this adhesive system is presented in a separate bottle) was applied actively for 10 s. After that the bond was applied on the etched and modified dentin by the primer. Then the adhesive was light cured for 20 s (18 J/cm2) (Radii, SDI, Australia).
Presence of moisture in the dentin using Single Bond Universal (universal-moist)
This adhesive system eliminates the acidic etching, so after the smear-layer standardization the dentin was washed and gently dried using light air jets , maintaining its moisture of the dentin. The universal adhesive system was then applied actively for 10 s, and photoactivated for 20 s (18 J/cm2) (Radii, SDI, Australia).
Absence of moisture in the dentin using Single Bond Universal (universal-dry)
After the smear-layer standardization the dentin was washed and completely dried using light air jets, resulting in a dentin without the glow suggestive of moisture. The universal adhesive system was then applied actively for 10 s, and photoactivated for 20 s (18 J/cm2) (Radii, SDI, Australia).
Restorative composite insertion
Five silicon molds of 1 mm high and 1 mm of internal diameter were distributed through the dentin surface already prepared with the adhesive techniques described above. Increments of the restorative composite (Filtek Z350, 3M ESPE) were inserted inside of each mold and photopolymerized for 20 s. The restored teeth were storage for 24 h in distillated water at 37 °C.
After storage, each specimen was submitted to the microshear test on a universal testing machine (Kratos LKC3, USB, Brazil). The mold was carefully removed with a # 11 scalpel blade leaving only the composite increments. The assembly was fixed to the base of the universal mechanical testing machine and an orthodontic wire (diameter 0.25 mm)  was passed surrounding each composite cylinder near the adhesion area, then attached to the load cell of the testing machine and shear force was applied to each cylinder at a speed of 0.5 mm/min until fracture of the specimen. The data obtained in Newton (N) were recorded for the subsequent statistical analysis. The value obtained in Newton is related to the load and through this value we calculated the bond strength by dividing it by the adhered area (RU = N/a). Then we calculate the average of each tooth from the value of the microshear bond strength (μSBS).
Scanning electron microscopy
All specimens (n = 30) were sputtered with by gold and evaluated under 120× magnification using scanning electron microscopy. This magnification was selected aiming to observe the whole circumference of each adhesion surface.
Failure mode were classified as following: Adhesive failure: dentin visualization in the majority of the evaluated area; Cohesive failure: visualization of peaks and valleys, which represents the fracture of dentin or composite (no distinction were made between the substrates) in the majority of the evaluated area; Mixed failure: visualization of both failure mode described in approximately equal proportions of the evaluated area.
The data from bond strength were evaluated using ANOVA (one-way) and Tukey’s test. For both tests the global level of significance was 5%.
Means (standard deviation) for the bond strength (MPa)
Bond strength (MPa)
The aim of this study was to evaluate the micro shear bond strength in dentin of the universal adhesive system (universal bond), varying the moisture in the dentin during the adhesion technique. We know that adhesion in dentin is achieved through the process of formation of the hybrid layer, initially described by Nakabayashi and Hiranuama . The adhesive systems have undergone several evolutions until the present arrival of the universal adhesive systems, where its self-etching mechanism promotes a modification or dissolution of the smear layer thus allowing its incorporation into the formation of the hybrid layer .
Due to the rapid development of new products, in vitro assays have become indispensable for comparing the bond strength of the adhesives to the substrates. The commonly used tests are those of tensile, micro tensile and shear . The micro-shear test was chosen for this study considering their advantages: it allows multiple samples in the same tooth without the need of cutting the teeth, being therefore easier and cheaper, and specially do not induce stress in the interface during the process [18–20]. According to Zohairy et al. directly compare the results from tensile and shear is impractical, but both tests are capable of ranking materials properly .
The dentin moisture did not affect the bond strength when the universal system was used. This finding probably can be explained by the presence of the copolymer that is highly hydrophilic and the MDP molecule that improves the self-etching technique . The conventional three-step adhesive system, the Scotchbond Multi Purpose (3M espe), was used in the control group, where it was mandatory to condition the dentine with phosphoric acid prior to the application of the adhesive. It is of great importance that after the acid conditioning, the dentin presents moisture since the water, in adequate quantities, avoids the collaborative collagen fibrils preventing the infiltration of the adhesive system in the interfibrillar spaces and consequently obtaining a weak union between restorative material and Dental structure . In view of this, the exclusion of the dry Scotchbond Multi Purpose group was not significant since poor adhesion or even non-adhesion was expected in completely dry dentin.
The results of this study showed that there was no statistical difference between the groups (p = 0.056), allowing to state that regardless of the technique, the Single Bond Universal adhesive system showed micro-shear bond strength similar to the conventional adhesive. Few studies show bond strength comparing the two techniques for this adhesive system. Marchesi et al. conducted a study with the objective of evaluating the adhesive stability over time through the micro tensile test and observed that the Universal Single Bond used in both the self-etching mode, the condition and wash mode, and dentin wet or dry, exhibited similar bond strength values to the control group after 24 h storage in water, corroborating with the results of the present study .
Garcia et al. carried out a study with the objective of evaluating the bond strength of all-in-one adhesives on different substrates, and observed that after a week of storage, through the micro-cleavage test, there were no differences Between the Single Bond Universal and the control group, where the substrate was dentin . In another study, Thanaratikul et al., evaluated the bond strength in primary dentin for different universal adhesive systems in both the self-etching mode and the conditional mode and washed through the microcuts test, and observed that the Universal Single Bond Used in the condition and wash mode obtained results of union strength superior to the control group. In addition, the same adhesive used in the self-etching mode obtained results of bond strength similar to the control group .
As for failure mode, it was observed that majority of the failures found were adhesive-type, with about 91% of all failures, followed by fractures of the mixed type, with about 8% of the total and almost no failures of the cohesive type, equivalent to only 1% of the total failures and found only in the Universal Single Bond (control technique group).
The adhesive failures indicate a rupture of the bond at the dentin/composite interface, the cohesive fractures breaking the dentin or composite, while mixed-type fractures, indicate cohesive disruption in the composite and adhesive in the dentin . In the micro-shear test the load cell was aligned parallel to the adhesive interface so that an application of the force closest to this joint occurred, ensuring correct orientation of the shear forces . Therefore, the higher prevalence of adhesive fractures indicated that the bond strength of the specimens was analyzed and not the internal resistance of the material.
Based on the results of the present study it can be concluded that the dentin moisture did not affect the bond strength when the universal adhesive was used, which is a very important fact considering that the moisture is the main concern during adhesion procedures.
FVC and MADP contributed to the preparation of teeth and data acquisition; LMC and WCB contributed to the microscopy analyses; CVRT contributed to data acquisition and interpretation; WMJ and LCCB contributed to conception design, analysis and interpretation. All authors read and approved the final manuscript.
The authors thank to Technological Characterization Laboratory of Department of Mining and Petroleum, University of São Paulo (LCT-EPUSP) for SEM analyses; FAPESP process 2015/09222-1; and 3M ESPE for the donation of the material. Any institution acknowledged had no role in the development of the study, data analysis, interpretation or writing.
The authors declare that they have no competing interests.
Availability of data and materials
Consent for publication
This manuscript is not concurrently under consideration for publication in any other journal. All the named authors were involved in the work leading to the publication of the paper, and all the named authors have read the paper before it is submitted for publication.
Ethics approval and consent to participate
The research protocol was approved by the ethics committee of the University of Santo Amaro (Process No. 1.203.890) before the study started.
This research was supported by FAPESP (2015/09222-1). This institution had no role in the development of the study, data analysis, interpretation or writing.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Van Meerbeek B, De Munck J, Yoshida Y, Inoue S, Vargas M, Vijay P, Van Landuyt K, Lambrechts P, Vanherle G. Buonocore memorial lecture. Adhesion to enamel and dentin: current status and future challenges. Oper Dent. 2003;28:215–35.Google Scholar
- Isolan CP, Valente LL, Münchow EA, Basso GR, Pimentel AH, Schwantz JK, Silva AV, Moraes RR. Bond strength of a universal bonding agent and other contemporary dental adhesives applied on enamel, dentin, composite, and porcelain. Appl Adhes Sci. 2014;2:25.View ArticleGoogle Scholar
- Frankenberger R, Tayb FR. Self-etch vs etch-and-rinse adhesives: effect of thermo-mechanical fatigue loading on marginal quality of bonded resin composite restorations. Dent Mater. 2005;21:397–412.View ArticleGoogle Scholar
- Münchow EA, Valente LL, Bossardi M, Priebe TC, Zanchi CH, Piva E. Influence of surface moisture condition on the bond strength to dentin of etch-and-rinse adhesive systems. Braz Oral J Sci. 2014;13:182–6.View ArticleGoogle Scholar
- Gregoire G, Guignes P, Nasr K. Effects of dentine moisture on the permeability of total-etch and one-step self-etch adhesives. J Dent. 2009;37:691–9.View ArticleGoogle Scholar
- Guimarães LA, Almeida JCF, Wang L, D’Alpino PHP, Garcia FPC. Effectiveness of immediate bonding of etch-and-rinse adhesives to simplified ethanol-saturated dentin. Rest Dent. 2012;26:177–82.Google Scholar
- Ayar MK. A review of ethanol wet bonding: principles and techniques. Eur J Dent. 2016;10:155–9.View ArticleGoogle Scholar
- Single Bond Universal Adhesive, Technical Product Profile. http://www.3mespe.com.
- Anusavice KJP. Materiais dentários. Rio de Janeiro: Elsevier; 2013.Google Scholar
- Swift EJ. Bonding systems for restorative materials—a comprehensive review. Pediatr Dent. 1998;20:2.Google Scholar
- Scholtanus JD, Purwanta K, Dogan N, Kleverlaan CJ, Feilzer AJ. Microtensile bond strength of three simplified adhesive systems to caries-affected dentin. J Adhes Dent. 2010;12(4):273–8.Google Scholar
- Miranda WG, Placido E, Moura SK, Cardoso PE. Influence of postextraction substrate aging on the microtensile bond strength of a dental adhesive system. J Adhes Dent. 2005;7(3):193–6.Google Scholar
- Margvelashvili M, Goracci C, Beloica M, Papacchini F, Ferrari M. In vitro evaluation of bonding effectiveness to dentin of all-in-one adhesives. J Dent. 2010;38(2):106–12.View ArticleGoogle Scholar
- Sanches KFL, Lodovici E, Boaro LCC, Gonçalves F, LE Rodrigues Filho. Influence of pH cycling and mechanical loading on the resin-dentin microtensile bond strength. J Adhes Sci Technol. 2016;31:1386–94.View ArticleGoogle Scholar
- El Zohairy AA, Saber MH, Abdalla AI, Feilzer AJ. Efficacy of microtensile versus microshear bond testing for evaluation of bond strength of dental adhesive systems to enamel. Dent Mater. 2010;26(9):848–54.View ArticleGoogle Scholar
- Foong J, Lee K, Nguyen C, Tang G, Austin D, Ch’ng C, Burrow M, Thomas D. Comparison of microshear bond strengths of four self-etching bonding systems to enamel using two test methods. Aust Dent J. 2006;51:252–7.View ArticleGoogle Scholar
- Nakabayashi N, Hiranuama K. Effect of etchant variation on wet and dry dentin bonding primed with 4-META/acetone. Dent Mater. 2000;16:274–9.View ArticleGoogle Scholar
- Braga RR, Meira JBC, Boaro LCC, Xavier TA. Adhesion to tooth structure: a critical review of “macro” test methods. Dent Mater. 2010;26(2):e38–49.View ArticleGoogle Scholar
- Moszner N, Salz U, Zimmermann J. Chemical aspects of self-etching enamel–dentin adhesives: a systematic review. Dent Mater. 2005;21:895–910.View ArticleGoogle Scholar
- Van Meerbeek B, Yoshihara K, Yoshida Y, Mine A, De Munck J, Van Landuyt KL. State of the art of self-etch adhesives. Dent Mater. 2011;27:17–28.View ArticleGoogle Scholar
- Marchesi G, Frasseto A, et al. Adhesive performance of a multi-mode adhesive system. 1-year in vitro study. J Dent. 2014;42:603–12.View ArticleGoogle Scholar
- Garcia RN, et al. Resistência de união de adesivos all-in-one em diferentes substratos. Salusvita. 2016;35:27–40.Google Scholar
- Thanaratikul B. Self-etch or etch-and-rinse mode did not affect the microshear bond strength of a universal adhesive to primary dentin. Dent Mater. 2016;35:174–9.View ArticleGoogle Scholar
- Pazinatto RB. Avaliação da resistência adesiva de resina composta em dentina humana, empregando sistemas adesivos autocondicionantes e monocomponente: teste de microtração. Dent Press Est. 2006;3:16–30.Google Scholar
- Garcia FCP, D’Alpino PHP, Terada RSS, Carvalho RM. Testes mecânicos para a avaliação laboratorial da união resina/dentina. Rev Fac Odontol Bauru. 2002;10:118–27.Google Scholar